Global-local finite element analysis of riveted railway bridge connections for fatigue evaluation
B.M. Imam, T.D. Righiniotis & M.K. Chryssanthopoulos Faculty of Engineering and Physical Sciences, University of Surrey, UK
ABSTRACT: Recent studies have found that stringer-to-cross-girder connections in riveted railway bridges are susceptible to fatigue cracking. Fatigue damage in these connections is caused by secondary, deformation induced effects. These effects are difficult to interpret in terms of a single, applied stress descriptor, which is customarily used in an S-N assessment. In order to address this problem, and, following the work published recently by the authors (Imam et al. 2006, 2007), in this paper the results of a global-local finite element analysis of a riveted railway bridge are used within the context of the theory of critical distances (TCD). Here, using the TCD in the way proposed by Taylor (Bellett et al. 2005), fatigue damage is shown to con-verge upon mesh refinement. Comparisons of the TCD-based method with its more traditional, detail-specific S-N counterpart, reveal that the latter can underestimate fatigue damage in some cases by a factor of 3.5.
In the past few years, fatigue of riveted railway bridges connections has received considerable attention. A number of damaged cases have been reported for stringer-to-cross-girder connec-tions both in railway and highway bridges confirming that these details are susceptible to fatigue cracking (Al-Emrani 2002). Fatigue damage in these connections is caused by deformation in-duced secondary stresses which were not taken into account during the design of these bridges. This is because these secondary effects are, even today, often very difficult to analyse, requiring sophisticated models. In this respect, the best way of avoiding this type of fatigue damage in new bridges is good detailing. For existing bridges however, it is still a challenge to find practi-cal, yet accurate, models to assess the remaining life of these details.
All modern fatigue related codes of practice employ the S-N method for the fatigue assess-ment of bridge details (BS 5400 1980, AASHTO 1998). A specific class, which depends on ge-ometry and loading, is assigned to the bridge detail in question. The fatigue life of the detail is then estimated by using its code-specified S-N curve with the nominal stress applied to it. This method can be easily used in conjunction with tensile riveted details such as bottom flange-to-web connections in built-up beams, cover plates and gusset connections between the primary members of a bridge with hangers, diagonals and bracings. In such details, it is straightforward to identify the nominal stress to be used for fatigue calculations and, owing to a large number of fatigue tests carried out on such details, their S-N curves are well defined.
On the other hand, it is almost impossible to identify the nominal stress in stringer-to-cross-girder connections and this is due to their complex behaviour which involves secondary effects and depends on the interaction of different components such as rivets, angle clips and parts of the primary bridge members such as flanges and webs. Although few full-scale fatigue tests have been carried out in such connections (Abouelmaaty et al. 1999, Al-Emrani 2005), the test results were not expressed in a meaningful way on an S-N basis due to the above mentioned dif-ficulties.
These difficulties can be overcome by focusing on the local stresses in the vicinity of the stress concentrations, which explicitly take into account their effect, rather than having to iden-tify a nominal stress value and use it with code-specified S-N curves which implicitly account for stress concentration effects. Local stress distributions can nowadays be obtained with preci-sion by using the finite element (FE) method even for the most complex details and geometries. However, the maximum stress obtained at the point of stress concentration (notch tip) and the stress distribution around its vicinity is sensitive to the mesh size used in the FE model. Over-conservative predictions are obtained when fatigue damage is estimated using this maximum stress. During recent years, it has been proposed that rather than considering the maximum stress only, the entire stress distribution ahead of the stress concentration should be taken into account for fatigue damage calculations (Bellett et al. 2005). This theory, called the Theory of Critical Distances (TCD), was developed by Taylor and will be presented in more detail later in the paper.
In the past, the authors have employed the S-N method for the estimation of the fatigue dam-age of stringer-to-cross-girder connections (Imam et al. 2006). Through this global investiga-tion, which was carried out by using a crude FE model consisting exclusively of shell elements, all the connections in a typical, short-span, riveted railway bridge were ranked according to their estimated fatigue damage and, therefore, the most critical one identified. The authors have sub-sequently refined their global model in the region of the most critical connection using sub-modelling techniques and three-dimensional brick elements (Imam et al. 2007), as shown in Figure 1. The exact geometrical features and all the connection components such as rivets, angle clips and parts of the stringer and cross-girder webs were modelled in detail. Other features per-tinent to riveted connections such as the rivet clamping force and the friction between the con-nected parts were also explicitly accounted for. The results obtained from this global-local analysis were presented in a qualitative context since notch tip stresses were considered.
In this paper, the TCD is used in order to obtain fatigue damage estimates through the global-local model and compare them with the estimates obtained in the past through the global model and the S-N method (Imam et al. 2006). For this reason, the BS 5400 (1980) medium traffic trains are initially traversed over the bridge. Histories of the maximum principal stress are ob-tained at various critical locations within the connection. By using the TCD in conjunction with the plain (un-notched) material S-N curve and Miners rule, the different components of the connection are ranked according to their estimated fatigue damage. Therefore, the most critical hot-spots of the connection where fatigue cracking is most likely to occur are identified. The damage estimates obtained from this more refined model are compared to its global model counterpart. The effect of rivet clamping force on fatigue damage is also quantified.
2 THE THEORY OF CRITICAL DISTANCES (TCD)
According to the TCD, all the physical processes leading to crack initiation are assumed to take place within a finite area/volume ahead of the stress concentration, called the process zone. Therefore, the fatigue behaviour depends on the elastic stress distribution within that region and not on a single stress concentration at a single point, as postulated by the traditional theory. The size of the process zone can be identified using two material properties: the plain specimen fa-tigue limit 0 and the crack propagation threshold Kth. Within the context of the TCD, a criti-cal distance, which characterises the region within which stresses are to be considered, is de-fined as (Taylor 1999):
It has to be noted that, since Kth and 0 are both material properties, Equation 1 implies that L will also be a material property.
There are several ways of implementing the TCD, depending on the stresses considered for further calculations. The simplest ways are by considering the maximum principal stress at a single point (point method), a distance of L/2 from the notch tip, or by averaging the maximum principal stress along a distance of 2L (line method) (Bellett et al. 2005).Two additional options
of the TCD is to average the maximum principal stress over a semi-circular area (area method) or over a hemisphere (volume method) (Bellett et al. 2005), both centred at the tip of the notch and having a radius of 1.32L and 1.54L respectively.
Having established the characteristic stress by using one of the previously mentioned meth-ods, this is then compared with the Constant Amplitude Fatigue Limit (CAFL) of the plain (un-notched) material in order to determine whether fatigue failure will occur. Comparison of ex-perimental and analytical results on a wide range of notch geometries (circular holes, fillets etc.) and materials (steel, cast iron, aluminum) showed that the TCD is capable of predicting fatigue strength within an error margin of 20% (Taylor & Wang 2000, Susmel & Taylor 2003).
The TCD has been primarily employed to determine the CAFL of all types of stress concen-trations but it has also been verified being capable of estimating fatigue life under variable am-plitude loading as well (Taylor et al. 2000). This was achieved by using the characteristic stress in conjunction with Miners rule and the plain material S-N curve. Furthermore, the accuracy of the TCD for the fatigue assessment of welded joints (Taylor et al. 2002), under multiaxial stress conditions (Susmel 2004) and for fretting fatigue problems (Araujo et al. 2007) has also been verified.
Following this brief discussion on the TCD, the FE analysis is presented in the next section. In this investigation, the TCD is used in conjunction with variable amplitude loading resulting from the passage of trains over a short-span, riveted bridge in order to estimate the fatigue dam-age and the remaining life of a critical connection. Due to the three-dimensional nature of the notches in the connection, the volume method of the TCD is employed.